A Prolific Solvate Former, Galunisertib, under the Pressure of Crystal Structure Prediction, Produces Ten Diverse Polymorphs.
Bhardwaj, Rajni M.; McMahon, Jennifer A.; Nyman, Jonas; Price, Louise S.; Konar, Sumit; Oswald, Iain D. H.; Pulham, Colin R.; Price, Sarah L.; Reutzel-Edens, Susan M; Journal of the American Chemical Society 141 (2019) 13887–13897; doi:10.1021/jacs.9b06634

data_4128840
_publ_section_title
;
 A Prolific Solvate Former, Galunisertib, under the Pressure of Crystal
 Structure Prediction, Produces Ten Diverse Polymorphs.
;
_journal_issue                   35
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              13887
_journal_page_last               13897
_journal_paper_doi               10.1021/jacs.9b06634
_journal_volume                  141
_journal_year                    2019
_chemical_formula_sum            'C22 H19 N5 O'
_chemical_formula_weight         369.42
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-2018/3
_cell_angle_alpha                102.001(10)
_cell_angle_beta                 105.368(11)
_cell_angle_gamma                102.349(9)
_cell_formula_units_Z            2
_cell_length_a                   8.2116(11)
_cell_length_b                   11.5104(14)
_cell_length_c                   11.8746(18)
_cell_measurement_reflns_used    2133
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      70.56
_cell_measurement_theta_min      4.023
_cell_volume                     1014.6(3)
_computing_cell_refinement       'SAINT 7.46A (Bruker-AXS, 2011)'
_computing_data_collection       'APEX2 v2011.4.0 (Bruker-AXS, 2011)'
_computing_data_reduction        'SAINT 7.46A (Bruker-AXS, 2011)'
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_structure_solution    'SHELXT (Sheldrick, 2015)'
_diffrn_ambient_temperature      100(2)
_diffrn_detector_area_resol_mean 10.4
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.978
_diffrn_measurement_device_type  'Bruker Photon 100 CMOS'
_diffrn_measurement_method       '\f and \w scans'
_diffrn_radiation_monochromator  'Incoatec I\mS multilayer optics'
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54178
_diffrn_reflns_av_R_equivalents  0.2796
_diffrn_reflns_av_unetI/netI     0.1820
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.978
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            21129
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.978
_diffrn_reflns_theta_full        25.000
_diffrn_reflns_theta_max         72.693
_diffrn_reflns_theta_min         4.023
_diffrn_source                   'I\mS micro-focus sealed tube'
_exptl_absorpt_coefficient_mu    0.623
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Sheldrick, 2009)'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.209
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       blade
_exptl_crystal_F_000             388
_exptl_crystal_size_max          0.274
_exptl_crystal_size_mid          0.039
_exptl_crystal_size_min          0.013
_exptl_transmission_factor_max   0.7535
_exptl_transmission_factor_min   0.5823
_refine_diff_density_max         1.120
_refine_diff_density_min         -0.413
_refine_diff_density_rms         0.114
_refine_ls_extinction_coef       0.0132(18)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2018/3 (Sheldrick 2018)'
_refine_ls_goodness_of_fit_ref   1.027
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     255
_refine_ls_number_reflns         3946
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.027
_refine_ls_R_factor_all          0.2542
_refine_ls_R_factor_gt           0.1506
_refine_ls_shift/su_max          0.017
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.1017P)^2^+7.0958P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.3149
_refine_ls_wR_factor_ref         0.3669
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1847
_reflns_number_total             3946
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            ja9b06634_si_001.cif
_cod_data_source_block           Galunisertib_FORM_II
_cod_database_code               4128840
_shelx_shelxl_version_number     2018/3
_shelx_estimated_absorpt_t_min   0.848
_shelx_estimated_absorpt_t_max   0.992
_shelx_res_checksum              74009
_shelx_hkl_checksum              8626